A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE


 Erin Todd
 1 years ago
 Views:
Transcription
1 A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering, The University of Manchester, Manchester M6 QD, U.K. SUMMARY Strain induced damage modes and their interactions are modelled using the finite element method for CMC tows and º/9º laminates. For both situations, biaxial straining is addressed, together with the degradation of Young s moduli and Poisson s ratios. In all cases, the expected stressstrain behaviour is predicted. Keywords: CMCs; Tows; Finite Element Method; Damage Mechanisms; Orthotropic Material; Constitutive Equations INTRODUCTION The superior material properties of Ceramic Matrix Composites (CMCs), e.g. low density and good mechanical and thermal properties at high temperatures make them favourable materials for use in: rocket nozzles; thermal protection systems; and gas turbine engines []. To perform optimal design of these engineering components, a highly efficient yet computational accurate model is a necessary requirement, due to the complex spatial topology and interactive damage mechanisms of woven CMCs. A finite element (FE) model of a unit cell geometry is a commonly used approach to study the behaviour of CMCs. Sheikh et al. [] employed a microstructural FE model to predict steadystate and transient heat conduction for the plain weave DLRXT composite. Deepak and Whitcomb [] evaluated load flow in plain weave composites by using a detailed D FE model and a nonstandard postprocessing technique. Although the full FE analysis is capable of predicting accurate micromechanical responses, it is computationally expensive because a precise description of the geometry is required. In order to tackle practical problems in the design and analysis of composites, some computationally efficient FE models have been developed. Tanov and Tabiei [4] predicted the equivalent material properties of plain weave fabric composites by homogenising an entire unit cell model. Cox et al. [5] introduced a Binary Model, which is composed of two virtual components: a D truss element and a D solid element. Whilst the Binary Model has great simplicity, it does require accurate determination of the mechanical and thermal properties of the two virtual components.
2 However, an alternative simpler and more accurate approach has been adopted here. For all of these approaches, the material properties are assumed to be linear elastic. The present paper addresses the development of a conceptually simple and computationally economic FE model, which emphasises the effects of straininduced damage modes and their interactions on the mechanical behaviour. Nonlinear material properties are modelled by multilinear elastic discretisation. A unidirectional tow is homogenised to a single orthotropic block. Multiaxial stressstrain response and degradation of material properties are modelled for unidirectional tows and º/9º laminates. BC: Matrix cracks CD & DE: (e) Wake debonding Matrix σ D Fibre A B C E CD & DE: Fibre rupture (f) DE: Fibre pullout (g) ν ν B D Figure. Schematic drawings of A unidirectional tow under longitudinal extension; and Longitudinal stressstrain and Poisson s ratiostrain curves; and (g) Corresponding damage modes. Poisson's ratio.... Experiment Idealisation Longitudinal strain Figure. Measured [8] and assumed variation of Poisson s ratios, ν and ν with longitudinal strain. DAMAGE MODES AND MECHANICAL BEHAVIOUR OF A UNI DIRECTIONAL TOW The damage modes and typical mechanical behaviour of a unidirectional tow subjected to different loading conditions are described in this section. The interactions of different damage modes and their effects on the stressstrain response are introduced.
3 Longitudinal extension When a unidirectional fibrereinforced ceramic matrix composite tow (single bundle of fibres and associated matrices) is under uniform extension along the fibre direction (Figure a), the typical longitudinal stressstrain response [5] (Figure b) and Poisson s ratiolongitudinal strain curve (Figure c), can be observed. The four characteristic stages in the stressstrain curve are now described [7]: AB: initially, the composite behaves as a virgin, undamaged, linear elastic material; BC: periodic matrix cracking occurs (Figure d); CD: fibrematrix interface debonding takes place at the matrix crack tip and its wake (wake debonding in Figure e); and weaker fibres fail (Figure f); DE: the majority of fibres fail and are pulled out against the frictional stress along the wake debonding interface (Figure g). Figure shows how the Poisson s ratiolongitudinal strain curve in Figure c can be idealised from the experimental data [8] for a unidirectional Nicalon/CAS composite. It can be seen that initially, Poisson s ratio is constant, then decreases linearly due to matrix cracking and wake debonding, and finally approaches zero at peak stress D, as shown in Figure b. σ A ν A B C B C To or Fibre Matrix debonding and/or matrix cracks (f) Figure. Schematic drawings of A unidirectional tow under transverse straining; and Transverse stressstrain and Poisson s ratio curves; and (f) Corresponding damage modes. γ γ τ A C B γ γ γ γ Fibre Matrix debonding and/or matrix cracks γ or (e) Figure 4. Schematic drawings of A unidirectional tow under shear straining; and Shear stressstrain curve; and (e) Corresponding damage modes.
4 Transverse extension When a unidirectional tow is subjected to transverse extension (Figure a), the material response is assumed to be piecewise linear elastic (Figure b and c). When the global transverse strain reaches a critical value, fibrematrix debonding and/or matrix cracking (Figure d f) is assumed to take place which leads to catastrophic failure. Shear loading As can be seen from Figure 4, in the case of shear straining, the shear stressstrain response and damage modes are assumed to have the same form as those for transverse straining. σ W Original N N W T W w w Nopullout Original Idealised Figure 5. Schematic drawing of Nopullout stressstrain curve; Variation of the normalised number of wake debonded blocks with longitudinal strain. Damage interactions and nopullout curve When a unidirectional tow is under multiaxial loading, e.g. both longitudinal and transverse straining ( and ); or both longitudinal and shear straining ( and γ ), the interaction between certain damage modes is strong and needs to be considered. The positive transverse stress ( σ ) or shear stress ( τ ) advances wake debonding, and hence decouples the interaction between fibres and matrix. As a result, the contribution due to fibre pullout has to be deactivated. Figure 5a shows that the original stressstrain curve degrades to the nopullout curve due to this damage interaction [5]. The damage interaction results in the change of Poisson s ratios. The broken curve in Figure 5b represents the variation of the normalised number of wake debonded blocks (fibrematrix between adjacent matrix cracks) in a tow with longitudinal strain [7]. In the present model, it is assumed that all the blocks wake debond at the point, W, viz. the dash curve in Figure 5b is idealised to the solid curve. The strain level at which the deactivation point W occurs has been determined by examination of the original and nopullout curves (Figure 5a). Consequently, Poisson s w ratios ν and ν drop to zero at the wake debonding strain,, when the switch to the nopullout curve is activated.
5 FORMULATION OF THE FINITE ELEMENT MODEL A unidirectional tow is chosen to be the basic constituent in the FE model, and therefore an entire tow, which consists of thousands of fibres embedded in matrix, can be represented by a single 8node solid finite element (Figure 6). The material properties are assumed to be multilinear elastic and the stressstrain and Poisson s ratiosstrain curves shown in Figures, and 4 are used to develop the constitutive equations. The FE package ABAQUS [9] with a userdefined subroutine UMAT is used to carried out the simulation. Tow Orthotropic Block This method has the benefit of being able to model a tow by a single orthotropic finite element. The approach has the advantage of simplicity relative to the binary system of modelling [5], since it has only one component; and, unlike the binary method, does not suffer from the difficulties associated with the identification of medium properties. Homogenisation of a unidirectional tow A heterogeneous unidirectional tow is homogenised to a single block (Figure 6), which has the same overall dimensions and equivalent orthotropic material properties. There are nine independent material properties: Young s moduli: E, E, and E ; Poisson s ratios: ν, ν, and ν ; Shear moduli: G, G, and G. Figure 6. Homogenisation of a unidirectional tow to a single orthotropic block. Discretisation of the stressstrain curve and constitutive equations In order to perform a finite element analysis, the nonlinear longitudinal stressstrain relationship is discretised to a multilinear curve. The loading is imposed in terms of the displacement boundary conditions, i.e. displacement controlled rather than load controlled conditions are modelled. The applied displacement is divided into many small increments. For each increment, the constitutive equations for an orthotropic material are: ν ν σ E E ν + ν ν σ E E σ = ν + ν ν τ EE τ τ ν + ν ν EE νν EE ν + νν EE ν + ν ν EE ν + νν EE νν EE G G γ γ γ G ()
6 ( ν ν ν ν νν ν ν ν ) E where = and ν i ij = ν ji (i, j = and i j). E E E E Assumptions of mechanical couplings due to damage interactions To model the interactions of the different damage modes, the following assumptions are made.. The switch from the original stressstrain curve to the nopullout curve is triggered by a small finite positive transverse stress, or by a small nonzero shear stress in the  or  plane.. Consequently, the Poisson s ratios, ν and ν drop to zero at the wake debonding strain, (Figure 5). w UMAT implementation in ABAQUS The present model is implemented by using the finite element package, ABAQUS/standard and a user defined subroutine, UMAT. The multilinear material properties, the constitutive equations, and the mechanical couplings are defined in the UMAT. For every increment, the UMAT reads the strains at each material point and then assigns the corresponding Young s moduli, Poisson s ratios and shear moduli. The constitutive equations are then used to update the stress fields. Solutiondependent state variables, STATEV, record different damage modes and control their interactions. Automatic incrementation algorithms and increment redefinition variable, PNEWDT, are continuously updated to ensure that the discretised points are located exactly at the end of the relevant increments. j MULTIAXIAL TOW AND º/9º LAMINATE BEHAVIOUR ( w,σ w ) σ σ D Wake debonding Longitudinal strain σ or σ Transverse strain or Poisson's ratio. ν. ν ν strain γ τ or γ τ γ τ Shear strain Figure 7. Material properties of a unidirectional tow.
7 The current model is used to analyse a unidirectional tow and a º/9º laminate under different loading cases. Applications to composite woven unit cells and real engineering components will be pursued as future developments. Material properties The material properties of a unidirectional tow of C/CSiC (Carbon/CarbonSilcon Carbide) DLRXT composite are shown in Figure 7. Figure 7a, which is associated with Figure 5a, has been obtained by using the model for a unidirectional tow [7]. The solid curve is the original longitudinal stressstrain relationship, the broken line defines the nopullout curve, and the cross symbol is the wake debonding point. The initial values of other properties, transverse moduli (Figure 7b), Poisson s ratios (Figure 7c), and shear moduli (Figure 7d) have been calibrated by a fully meshed micromechanical FE model. The limit of proportionality of the experimental stressstrain curve for the DLR XT material under uniaxial straining, is used to define a transverse failure strain of.4% []. A value of 6MPa is used to determine the critical shear failure strain []. Poisson's ratio Strain Longitudinal strain σ ν ν Poisson's ratio Strain Transverse strain σ ν ν Figure 8. Finite element results for a unidirectional tow under longitudinal straining ( ). Figure 9. Finite element results for a unidirectional tow under transverse straining ( ) Shear strain γ γ τ Figure. Finite element results for a unidirectional tow under shear straining.
8 Unidirectional tow: longitudinal, transverse and shear straining Figure 8 shows the FE results for a unidirectional tow under longitudinal straining. The stressstrain relationship, longitudinaltransverse strain curves, and variation of Poisson s ratios are plotted in Figure 8a, 8b, and 8c, respectively. As expected, the results are identical to the defined material properties. The results for a unidirectional tow subjected to transverse and shear straining are presented in Figures 9 and, respectively. Once again, the method has been validated since input and output values concur. Strain Strain ratio σ σ ( / ) Strain Strain ratio σ τ ( / ) ( / ) Longitudinal strain Longitudinal strain Figure. Finite element results for a unidirectional tow under equibiaxial straining ( = ). Figure. Finite element results for a unidirectional tow under longitudinal straining ( ) and shear straining (γ ) with =γ. Unidirectional tow: equibiaxial straining Figure shows the FE results for a tow under equibiaxial tensile straining, =. From Figure a, it can be seen that the nopullout stressstrain curve is triggered due to the positive stress σ. Figure b shows that the transverse stress, σ drops to zero at the defined failure strain ( =.4%). The effect of this transverse failure on the deformation in the other transverse direction is shown as a kink in Figure c. The
9 effect can also be seen from the first sharp drop in Figure d, which plots the ratio of strains in Figure c. The second sharp drop in Figure d is due to the second assumption of mechanical coupling, namely that the Poisson s ratio drops to zero at the wake debonding strain. Unidirectional tow: combined longitudinal and shear straining In comparison with the predictions for equibiaxial straining, similar results are obtained for longitudinal and shear straining (Figure ). In this case, the switch from original to nopullout curve is triggered by the shear stress. Transverse strains become zero at the wake debonding strain. º tows 9º tows Strain Composite strain σ Figure. Schematic drawing of a º/9º tow laminate under uniaxial straining Figure 4. Overall behaviour of a º/9º laminate under uniaxial straining Composite strain σ 9 σ Composite strain σ 9 σ Figure 5. Local behaviour of a º/9º laminate under uniaxial straining.
10 º/9º laminate under uniaxial straining, The model is also used to analyse a º/9º laminate under inplane uniaxial straining (Figure ). The overall stressstrain response and variations of transverse strains are shown in Figure 4a and 4b, respectively. The kinks at =.4% in both figures are due to the matrix cracking in the 9º tows. The transverse strains drop to zero at the wake debonding strain,. w Figures 5 show the longitudinal stressstrain and transverse stressstrain response in the different layers. As can be seen from Figure 5a, the nopullout curve is triggered in the º layer. This is because the º layer carries a transverse tensile stress (Figure 5c) before the wake debonding strain is reached. This tensile stress is created by the constraint of the 9º layer, since its stiffness in the direction is much higher than that of the º layer. In order to satisfy equilibrium, the transverse stress in the 9º layer (Figure 5d) is a mirror of that given in Figure 5c. According to this analysis, even though a º/9º laminate is only under inplane uniaxial tension, the nopullout curve can still be activated. This is different to the stressstrain response of longitudinal straining of a unidirectional tow. DISCUSSION AND CONCLUSIONS A computationally efficient FE model has been developed to predict the mechanical behaviour of ceramic matrix composites with straininduced damage. The effects of different damage modes and their interactions on mechanical behaviour have been considered. The basic constituent of the FE model is an orthotropic 8node brick, which forms a homogenised medium of a heterogeneous unidirectional tow. The nonlinear longitudinal material properties are discretised to a multilinear elastic curve. The constitutive equations for orthotropic materials are used to update the stresses for each increment of the analysis. The model is implemented by a commercial FE package, ABAQUS with a user defined subroutine, UMAT. Multiaxial stressstrain response and degradation of material properties have been modelled for a unidirectional tow, and for a º/9º laminate. In all analyses, the expected mechanical behaviour has been obtained. For the º/9º laminate under uniaxial straining, the nopullout stressstrain response in the º layer is triggered due to the constraint of the 9º layer. The high efficiency and the simplicity of the model make it possible to analyse large scale woven composites. Application of the model to unit cells and to real engineering components will be pursued as future developments. ACKNOWLEDGEMENTS Matthew Blacklock is gratefully acknowledged for providing the material properties used in this paper; and, for ongoing discussions.
11 References. Marshall, D. B. and Cox, B. N. 8 Integral textile ceramic structures. Annu. Rev. Mater. Res., 8, Sheikh, M. A., Taylor, S. C., Hayhurst, D. R. and Taylor, R. Microstructural finite element modelling of a ceramic matrix composite to predict experimental measurements of its macro thermal properties. Model. Simul. Mater. Sci. Eng. 9, 7.. Deepak, G. and Whitcomb, J. D. 8 Load flow in plain woven composites. Journal of Composite Materials. 4, Tanov, R. and Tabiei, A. Computationally efficient micromechanical models for woven fabric composite elastic moduli. Journal of Applied Mechanics. 68, Cox, B. N., Carter, W. C., and Fleck, N. A. 994 A binary model of textile composites I. Formulation. Acta Metall. Mater. 4, Hayhurst, D. R., Leckie, F. A. and Evans, A. 99 Component designbased model for deformation and rupture of tough fibrereinforced ceramic matrix composites. Proc. R. Soc. Lond. A. 44, Tang, C., Blacklock, M, and Hayhurst, D. R. 8 Thermomechanical behaviour of Ceramic Matrix Composites: Part I Stressstrain response and thermal conductivity degradation of fibre tows. Research report No. DMM. 8.4, School of Mechanical, Aerospace and Civil Engineering, The University of Manchester, U.K. 8. Karandikar, P. and Chou, T. 99 Characterization and modelling of microcracking and elastic moduli changes in Nicalon/CAS composites. Composites Science and Technology. 46, SIMULIA. 6 ABAQUS user s manual. Version Sheikh, M. A., Hayhurst, D.R., Taylor, S. C. and Taylor, R. 7 Experimental Investigation of the effect of mechanical loading on Thermal Transport in Ceramic Matrix Composites Research report No. DMM. 8.6, School of Mechanical, Aerospace and Civil Engineering, The University of Manchester, U.K.. Tang, C., Blacklock, M, and Hayhurst, D. R. 8 Thermomechanical behaviour of Ceramic Matrix Composites: Part II Stressstrain response and thermal conductivity degradation of fibre tows, 9 unidirectional and woven composites. Research report No. DMM. 8.5, School of Mechanical, Aerospace and Civil Engineering, The University of Manchester, U.K.
Stressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension, compression or shear
Xi an 225 th August 217 Stressstrain response and fracture behaviour of plain weave ceramic matrix composites under uniaxial tension compression or shear Heyin Qi 1 Mingming Chen 2 Yonghong Duan 3 Daxu
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationComposite models 30 and 131: Ply types 0 and 8 calibration
Model calibration Composite BiPhase models 30 and 3 for elastic, damage and failure PAMCRASH material model 30 is for solid and 3 for multilayered shell elements. Within these models different ply types
More informationAn orthotropic damage model for crash simulation of composites
High Performance Structures and Materials III 511 An orthotropic damage model for crash simulation of composites W. Wang 1, F. H. M. Swartjes 1 & M. D. Gan 1 BU Automotive Centre of Lightweight Structures
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationMULTISCALE MODELLING OF FIBRE BUNDLES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MULTISCALE MODELLING OF FIBRE BUNDLES N. D. Chakladar 1, P. Mandal 1 *, P. Potluri 2 1 School of Mechanical, Aerospace and Civil Engineering,
More informationMeasurement of mesoscale deformations for modelling textile composites
CompTest 2004 Measurement of mesoscale deformations for modelling textile composites P Potluri, D A Perez Ciurezu, R Ramgulam Textile Composites Group University of Manchester Institute of Science & Technology
More informationNumerical Analysis of Composite Panels in the PostBuckling Field taking into account Progressive Failure
Copyright c 007 ICCES ICCES, vol.1, no.3, pp.9398, 007 Numerical Analysis of Composite Panels in the PostBuckling Field taking into account Progressive Failure C. Bisagni 1 Summary The research here
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More informationMultiscale Approach to Damage Analysis of Laminated Composite Structures
Multiscale Approach to Damage Analysis of Laminated Composite Structures D. Ivančević and I. Smojver Department of Aeronautical Engineering, Faculty of Mechanical Engineering and Naval Architecture, University
More informationDiscrete Element Modelling of a Reinforced Concrete Structure
Discrete Element Modelling of a Reinforced Concrete Structure S. Hentz, L. Daudeville, F.V. Donzé Laboratoire Sols, Solides, Structures, Domaine Universitaire, BP 38041 Grenoble Cedex 9 France sebastian.hentz@inpg.fr
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationNumerical analysis of the mechanical response of wood glulam beams reinforced through the thickness by FRP rods.
Numerical analysis of the mechanical response of wood glulam beams reinforced through the thickness by FRP rods. Giuseppe Giambanco 1, Tiziana Turetta 1, Alessia Cottone 1 1 Department of Structural, Aerospace
More informationMost of the material in this package is based on a recently published book. This is:
Mechanics of Composite Materials Version 2.1 Bill Clyne, University of Cambridge Boban Tanovic, MATTER Assumed Preknowledge It is assumed that the student is familiar with simple concepts of mechanical
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationPowerful Modelling Techniques in Abaqus to Simulate
Powerful Modelling Techniques in Abaqus to Simulate Necking and Delamination of Laminated Composites D. F. Zhang, K.M. Mao, Md. S. Islam, E. Andreasson, Nasir Mehmood, S. KaoWalter Email: sharon.kaowalter@bth.se
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More informationCalculation of Damagedependent Directional Failure Indices from the TsaiWu Static Failure Criterion
Van Paepegem, W. and Degrieck, J. (3. alculation of Damagedependent Directional Failure Indices from the saiwu Static Failure riterion. omposites Science and echnology, 63(, 353. alculation of Damagedependent
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationMultiscale analyses of the behaviour and damage of composite materials
Multiscale analyses of the behaviour and damage of composite materials Presented by Didier BAPTISTE ENSAM, LIM, UMR CNRS 8006 151 boulevard de l hôpital l 75013 PARIS, France Research works from: K.Derrien,
More informationTowards Affordable, ClosedLoop Recyclable Future Low Carbon Vehicles. Supervisors : Dr. L.T. Harper, Dr. M. Johnson, Prof. N.A.
Towards Affordable, ClosedLoop Recyclable Future Low Carbon Vehicles Supervisors : Dr. L.T. Harper, Dr. M. Johnson, Prof. N.A. Warrior Moulding issues with CF/PP Now looking to use CF/PA6 consolidation
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationInfluence of fibre proportion and position on the machinability of GFRP composites An FEA model
Indian Journal of Engineering & Materials Sciences Vol. 12, October 2005, pp. 443450 Influence of fibre proportion and position on the machinability of GFRP composites An FEA model D Abdul Budan* Department
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationBRIDGING LAW SHAPE FOR LONG FIBRE COMPOSITES AND ITS FINITE ELEMENT CONSTRUCTION
Proceedings of ALGORITMY 2012 pp. 353 361 BRIDGING LAW SHAPE FOR LONG FIBRE COMPOSITES AND ITS FINITE ELEMENT CONSTRUCTION VLADISLAV KOZÁK AND ZDENEK CHLUP Abstract. Ceramic matrix composites reinforced
More informationModule 7: Micromechanics Lecture 34: Self Consistent, Mori Tanaka and Halpin Tsai Models. Introduction. The Lecture Contains. Self Consistent Method
Introduction In this lecture we will introduce some more micromechanical methods to predict the effective properties of the composite. Here we will introduce expressions for the effective properties without
More informationFinite Element Method in Geotechnical Engineering
Finite Element Method in Geotechnical Engineering Short Course on + Dynamics Boulder, Colorado January 58, 2004 Stein Sture Professor of Civil Engineering University of Colorado at Boulder Contents Steps
More informationAbstract. 1 Introduction
Contact analysis for the modelling of anchors in concrete structures H. Walter*, L. Baillet** & M. Brunet* *Laboratoire de Mecanique des Solides **Laboratoire de Mecanique des ContactsCNRS UMR 5514 Institut
More informationUniversity of Sheffield The development of finite elements for 3D structural analysis in fire
The development of finite elements for 3D structural analysis in fire Chaoming Yu, I. W. Burgess, Z. Huang, R. J. Plank Department of Civil and Structural Engineering StiFF 05/09/2006 3D composite structures
More informationAn integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale
An integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale Angelos Mintzas 1, Steve Hatton 1, Sarinova Simandjuntak 2, Andrew Little 2, Zhongyi
More informationImpact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics
Impact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics Dr. A. Johnson DLR Dr. A. K. Pickett ESI GmbH EUROPAM 99 Impact and Crash Modelling of Composite Structures: A Challenge
More informationA Stress Gradient Failure Theory for Textile Structural Composites. Final Technical Report submitted to ARO
A Stress Gradient Failure Theory for Textile Structural Composites Final Technical Report submitted to ARO By RYAN KARKKAINEN and BHAVANI SANKAR University of Florida Department of Mechanical & Aerospace
More informationSupplementary Figures
Fracture Strength (GPa) Supplementary Figures a b 10 R=0.88 mm 1 0.1 Gordon et al Zhu et al Tang et al im et al 5 7 6 4 This work 5 50 500 Si Nanowire Diameter (nm) Supplementary Figure 1: (a) TEM image
More informationCHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement
CHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement Mark Hughes 19 th September 2016 Outline Fibre architecture Volume fraction and the rule of mixtures Principle
More informationCombined IsotropicKinematic Hardening Laws with Anisotropic Backstress Evolution for Orthotropic FiberReinforced Composites
Combined IsotropicKinematic Hardening Laws with Antropic Backstress Evolution for Orthotropic Fiber Reinforced Composites Combined IsotropicKinematic Hardening Laws with Antropic Backstress Evolution
More informationPrediction of Micromechanical Behaviour of Elliptical Frp Composites
Prediction of Micromechanical Behaviour of Elliptical Frp Composites Kiranmayee.Nerusu Dept. of Mechanical Engg. P. V. P. Siddhartha Institute of Technology, Vijayawada 520 007, A.P, India. P. Phani Prasanthi
More informationScienceDirect. Unit cell model of woven fabric textile composite for multiscale analysis. Anurag Dixit a *,Harlal Singh Mali b, R.K.
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 68 ( 2013 ) 352 358 The Malaysian International Tribology Conference 2013 (MITC2013) Unit cell model of woven fabric textile
More informationNonlinearities in mechanical behavior of textile composites
Composite Structures 71 (25) 61 67 www.elsevier.com/locate/compstruct Nonlinearities in mechanical behavior of textile composites Enrico DÕAmato Energetics Departement, L Aquila University, 674 Monteluco
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationANALYSIS OF LOAD FLOW AND STRESS CONCENTRATIONS IN TEXTILE COMPOSITES
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS ANALYSIS OF LOAD FLOW AND STRESS CONCENTRATIONS IN TEXTILE COMPOSITES Deepak Goyal*, John D. Whitcomb*, Julian Varghese* *Department of Aerospace Engineering,
More informationOverview of Probabilistic Modeling of Woven Ceramic Matrix Composites ABSTRACT
ABSTRACT An overview of current research efforts in understanding the cause of variability in the thermomechanical properties of woven ceramic matrix composites is presented. Statistical data describing
More informationKeywords: computer aided engineering, finite element analysis, multi scale modelling, fatigue life prediction
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS 3D TEXTILE COMPOSITE MECHANICAL PROPERTIES Jonathan J. Crookston, Sreedhar Kari, Nicholas A. Warrior, I. Arthur Jones & Andrew C. Long University of
More informationA STRAINBASED DAMAGE MECHANICS MODELING FOR WOVEN FABRIC COMPOSITES UNDER BIAXIAL FATIGUE LOADING
International Journal of Civil Engineering and Technology (IJCIET) Volume 9, Issue 3, March 2018, pp. 282 291, Article ID: IJCIET_09_03_030 Available online at http://http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=9&itype=3
More informationDevelopment of a Progressive Failure Model for Notched Woven Composite Laminates. Daniel Christopher Munden
Development of a Progressive Failure Model for Notched Woven Composite Laminates Daniel Christopher Munden Thesis submitted to the faculty of the Virginia Polytechnic Institute and State University in
More informationFracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load
Fracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load Sriram Chintapalli 1, S.Srilakshmi 1 1 Dept. of Mech. Engg., P. V. P. Siddhartha Institute of Technology.
More informationMODELLING OF THE THERMOMECHANICAL PROPERTIES OF WOVEN COMPOSITES DURING THE CURE
TH 9 TH INTRNATIONAL ONFRN ON OMPOSIT MATRIALS MODLLING OF TH THRMOMHANIAL PROPRTIS OF WOVN OMPOSITS DURING TH UR L. Khoun,, K.S. hallagulla,, P. Hubert Department of Mechanical ngineering, McGill University,
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationTHE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS THE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES L.V. Smith 1 *, M. Salavatian 1 1 School of Mechanical and Materials
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationMICROMECHANICAL ANALYSIS OF WOVEN COMPOSITES USING VARIATIONAL ASYMPTOTIC METHOD
MICROMECHANICAL ANALYSIS OF WOVEN COMPOSITES USING VARIATIONAL ASYMPTOTIC METHOD Rajeev G. Nair 1,2, B. Sivasubramonian 2, P. J. Guruprasad 1 1 Department of Aerospace Engineering, Indian Institute of
More informationModeling and simulation of continuous fiberreinforced
Scholars' Mine Doctoral Dissertations Student Research & Creative Works 2014 Modeling and simulation of continuous fiberreinforced ceramic composites Venkata Bheemreddy Follow this and additional works
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationTHE INFLUENCE OF INPLANE DENSITY VARIATION ON ENGINEERING PROPERTIES OF ORIENTED STRANDBOARD: A FINITE ELEMENT SIMULATION
Proceedings of McMat5: 5 Joint ASME/ASCE/SES Conference on Mechanics and Materials June 13, 5, Baton Rouge, Louisiana, USA 255 THE INFLUENCE OF INPLANE DENSITY VARIATION ON ENGINEERING PROPERTIES OF
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More informationProgressive Failure Analysis of Plain Weaves Using Damage Mechanics Based Constitutive Laws
Progressive Failure Analysis of Plain Weaves Using Damage Mechanics Based Constitutive Laws M. Kollegal, S. N. Chatterjee and G. Flanagan Materials Sciences Corporation, 500 Office Center Drive, Suite
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationProgressive Damage of GFRP Composite Plate Under Ballistic Impact: Experimental and Numerical Study
Progressive Damage of GFRP Composite Plate Under Ballistic Impact: Experimental and Numerical Study Progressive Damage of GFRP Composite Plate Under Ballistic Impact: Experimental and Numerical Study Md
More informationTHE BEHAVIOUR OF REINFORCED CONCRETE AS DEPICTED IN FINITE ELEMENT ANALYSIS.
THE BEHAVIOUR OF REINFORCED CONCRETE AS DEPICTED IN FINITE ELEMENT ANALYSIS. THE CASE OF A TERRACE UNIT. John N Karadelis 1. INTRODUCTION. Aim to replicate the behaviour of reinforced concrete in a multiscale
More informationModelling of ductile failure in metal forming
Modelling of ductile failure in metal forming H.H. Wisselink, J. Huetink Materials Innovation Institute (M2i) / University of Twente, Enschede, The Netherlands Summary: Damage and fracture are important
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationMESOSCALE MODELLING IN THERMOPLASTIC 5HARNESS SATIN WEAVE COMPOSITE
MESOSCALE MODELLING IN THERMOPLASTIC 5HARNESS SATIN WEAVE COMPOSITE S. Daggumati a*,i. De Baere a, W. Van Paepegem a, J. Degrieck a, J. Xu b, S.V. Lomov b, I. Verpoest b a Ghent University, Dept. of
More informationAN LSDYNA USER DEFINED MATERIAL MODEL FOR LOOSELY WOVEN FABRIC WITH NONORTHOGONAL VARYING WEFT AND WARP ANGLE
7 th International LSDYNA Users Conference Material Technology (1) AN LSDYNA USER DEFINED MATERIAL MODEL FOR LOOSELY WOVEN FABRIC WITH NONORTHOGONAL VARYING WEFT AND WARP ANGLE Marlin Brueggert Romil
More informationStatic and Time Dependent Failure of Fibre Reinforced Elastomeric Components. Salim Mirza Element Materials Technology Hitchin, UK
Static and Time Dependent Failure of Fibre Reinforced Elastomeric Components Salim Mirza Element Materials Technology Hitchin, UK Introduction Fibre reinforced elastomers are used in many applications,
More informationCrashworthiness of Composite Structures with Various Fiber Architectures
11 th International LDYNA Users Conference Crash afety Crashworthiness of Composite tructures with Various Fiber Architectures Nageswara R. Janapala 1, FuKuo Chang, Robert K. Goldberg 3, Gary D. Roberts
More informationAn ElastoViscoPlastic Multiscale Model for Fibrous Unidirectional Composite Materials
An ElastoViscoPlastic Multiscale Model for Fibrous Unidirectional Composite Materials by Shari Lynn King A thesis presented to the University of Waterloo in fulfillment of the thesis requirement for
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationRandom FiberMatrix Model for Predicting Damage in Multiscale Analysis of Textile Composites under Thermomechanical Loads
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Random FiberMatrix Model for Predicting Damage in Multiscale Analysis of Textile Composites under Thermomechanical Loads W. R. McLendon, J. D.
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationPREDICTING THE CONSTITUTIVE BEHAVIOR OF BIAXIAL BRAIDED COMPOSITES USING BEAM UNIT CELLS
THE 19TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PREDICTING THE CONSTITUTIVE BEHAVIOR OF BIAXIAL 1 J. Cichosz1*, J. Bückle1, R. Hinterhölzl1, M. Wolfahrt2 Institute for Carbon Composites, Technische
More informationRESPONSE SURFACES OF MECHANICAL BEHAVIOR OF DRY WOVEN FABRICS UNDER COMBINED LOADINGS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS RESPONSE SURFACES OF MECHANICAL BEHAVIOR OF DRY WOVEN FABRICS UNDER COMBINED LOADINGS M. Komeili, A.S. Milani* School of Engineering, University
More informationMODELING DYNAMIC FRACTURE AND DAMAGE IN A FIBERREINFORCED COMPOSITE LAMINA WITH PERIDYNAMICS
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Mechanical & Materials Engineering Faculty Publications Mechanical & Materials Engineering, Department of 011 MODELING DYNAMIC
More informationStrength of GRPlaminates with multiple fragment damages
Strength of GRPlaminates with multiple fragment damages S. Kazemahvazi, J. Kiele, D. Zenkert Kungliga Tekniska Högskolan, KTH 100 44 Stockholm, Sweden sohrabk@kth.se SUMMARY The strength of glass fibre
More informationTransactions on Engineering Sciences vol 21, 1998 WIT Press, ISSN
Micromechanical modelling of textile composites using variational principles A. Prodromou, Ph. Vandeurzen, G. Huysmans, J. Ivens & I. Verpoest Department ofmetallurgy and Materials Engineering, Katholieke
More informationInfluence of uniaxial and biaxial tension on mesoscale geometry and strain fields in a woven composite
Composite Structures 77 (7) 45 418 www.elsevier.com/locate/compstruct Influence of uniaxial and biaxial tension on mesoscale geometry and strain fields in a woven composite P. Potluri *, V.S. Thammandra
More informationTOWARD VIRTUAL CERAMIC COMPOSITES
TOWARD VIRTUAL CERAMIC COMPOSITES M. Genet 1, P. Ladevèze 12, G. Lubineau 1 1 LMTCachan (ENSCachan, CNRS, Paris 6 University, UniverSud Paris PRES) 61 avenue du Président Wilson 94235 Cachan CEDEX {genet,
More informationModule4. Mechanical Properties of Metals
Module4 Mechanical Properties of Metals Contents ) Elastic deformation and Plastic deformation ) Interpretation of tensile stressstrain curves 3) Yielding under multiaxial stress, Yield criteria, Macroscopic
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationPROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING. C. G. Dávila, P. P. Camanho, and M. F. de Moura
PROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING C. G. Dávila, P. P. Camanho, and M. F. de Moura Abstract The debonding of skin/stringer constructions is analyzed using a stepbystep simulation
More informationConstitutive model for quasistatic deformation of metallic sandwich cores
INTERNATIONAL JOURNAL FOR NUMERICAL METHODS IN ENGINEERING Int. J. Numer. Meth. Engng 2004; 61:2205 2238 Published online 18 October 2004 in Wiley InterScience (www.interscience.wiley.com). DOI: 10.1002/nme.1142
More informationTransactions on Modelling and Simulation vol 10, 1995 WIT Press, ISSN X
Parameters controlling the numerical simulation validity of damageable composite toughness testing S. Yotte, C. Currit, E. Lacoste, J.M. Quenisset Laboratoire de Genie Meanique  IUT 'A\ Domaine Universitaire,
More informationFINITE ELEMENT ANALYSIS OF THE ELASTIC CONSTITUTIVE BEHAVIOR OF A 2.5D INTERLOCK COMPOSITE
FINITE ELEMENT ANALYSIS OF THE ELASTIC CONSTITUTIVE BEHAVIOR OF A 2.5D INTERLOCK COMPOSITE NEHME Samer *, HAGEGE Benjamin *, KAABI Abderrahmen **, BENZEGGAGH Malk * * Université de Technologie de Compiègne,
More informationComposites Science and Technology
Composites Science and Technology 7 (1) 194 1941 Contents lists available at ScienceDirect Composites Science and Technology journal homepage: www.elsevier.com/locate/compscitech Local damage in a 5harness
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More informationCOMPRESSIVE BEHAVIOR OF IMPACT DAMAGED COMPOSITE LAMINATES
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS COMPRESSIVE BEHAVIOR OF IMPACT DAMAGED COMPOSITE LAMINATES Hiroshi Suemasu*, Wataru Sasaki**, Yuuichiro Aoki***, Takashi Ishikawa**** *Department of
More informationDYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.1419:628.183=20 DYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES J. ESKANDARI JAM 1 and N. GARSHASBI NIA 2 1 Aerospace
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationNUMERICAL MODELING OF GAS LEAKAGE THROUGH DAMAGED COMPOSITE LAMINATES
NUMERICAL MODELING OF GAS LEAKAGE THROUGH DAMAGED COMPOSITE LAMINATES Hisashi Kumazawa*, John Whitcomb** [Hisashi Kumazawa]:kumazawa.hisashi@jaxa.jp *Structure Technology Center, Japan Aerospace Exploration
More information